     • date post

28-Jun-2018
• Category

## Documents

• view

213
• download

0

Embed Size (px)

### Transcript of Semiconductor Devices 26 - University of York ah566/lectures/semi26_schottky_  · 1 Department of...

• 1

Department of Electronics

Semiconductor Devices 26

Atsufumi Hirohata

11:00 Tuesday, 2/December/2014 (P/T 006)

Exercise 5

State the following metals in contact with Si to form either

Schottky or Ohmic contacts based on their energy

diagram. Assume the following parameters:

Si electron affinity: = 4.05 eV

and Si bandgap: Eg = 1.11 eV.

Metal Work function M [eV]

n-type Si

p-type Si

Pt 6.30

Au 4.80

Cu 4.18

Ni 4.01

• 2

Answer to Exercise 5 The electron affinity is defined as

For an n-type contact,

! = vacuum level( )!EC

!B = !M ! "

Metal Work function M [eV]

n-type Si p-type Si

Pt 6.30 Schottky contact B = eV

Ohmic contact M (= 6.30) > + Eg (= 4.05 + 1.11)

Au 4.80 Schottky contact B = eV

Schottky contact B = eV

Cu 4.18 Schottky contact B = 4.18 4.05 = 0.13 eV

Schottky contact B = 4.05 + 1.11 4.18 = 0.98 eV

Ni 4.01 Ohmic contact M (= 4.01) < (=4.05)

Schottky contact B = 4.05 + 1.11 4.01 = 1.15 eV

!M > "

!M < " : ( ) contact

: ( ) contact with the barrier height of

For an p-type contact,

!B = " +Eg !!M!M < " +Eg

!M > " +Eg : ( ) contact : ( ) contact with the barrier height of

Answer to Exercise 5

Metal Work function M [eV]

n-type Si p-type Si

Pt 6.30 Schottky contact B = 6.30 4.05 = 2.25 eV

Ohmic contact M (= 6.30) > + Eg (= 4.05 + 1.11)

Au 4.80 Schottky contact B = 4.80 4.05 = 0.75 eV

Schottky contact B = 4.05 + 1.11 4.80 = 0.36 eV

Cu 4.18 Schottky contact B = 4.18 4.05 = 0.13 eV

Schottky contact B = 4.05 + 1.11 4.18 = 0.98 eV

Ni 4.01 Ohmic contact M (= 4.01) < (=4.05)

Schottky contact B = 4.05 + 1.11 4.01 = 1.15 eV

Metal

n-type semiconductor

• 3

26 Schottky Junction

Image force Schottky effect

Depletion layer capacity Ohmic contact

Schottky Barrier Definition of energy at the Schottly barrier :

* S. M. Sze, Physics of Semiconductor Devices (Wiley, New York, 2006).

• 4

Image Force

* S. Kishino, Physics of Semiconductor Devices (Maruzen, Tokyo, 1995).

Origin of image force :

Metal (M) Vacuum

Force between the two electrons :

F =q ! "q( )

4!"0 2x( )2 Coulomb's law[ ]

Image Force at a Metal Semiconductor Interface

Potential energy for an electron :

E x( ) = F dx!

x" =

q # \$q( )4!"0 2x( )

2!

x" dx = \$ q

2

16!"0x2!

x" dx

=\$q2

16!"0#x\$2+1

\$2+1( )

%

&''

(

)**!

x

=q2

16!"0#1x

%

&'

(

)*!

x

=q2

16!"01x\$1!

+

,-

.

/0

=q2

16!"0xImage force at a metal semiconductor interface :

Vacuum level

Vacuum

* S. Kishino, Physics of Semiconductor Devices (Maruzen, Tokyo, 1995).

• 5

External Electric Field Application

Under an electric field E :

E x( ) = q2

16!"0x+ q!Ex

Schottky barrier at a metal semiconductor interface :

* S. Kishino, Physics of Semiconductor Devices (Maruzen, Tokyo, 1995).

Vacuum level

Vacuum

( ) effect

Metal - Semiconductor Junction Realistic energy diagram of a Schottky junction :

* S. Kishino, Physics of Semiconductor Devices (Maruzen, Tokyo, 1995).

Junction

Under a forward bias application : Under a reverse bias application :

• 6

Depletion Layer Capacity Under reverse bias, Poissons equation is defined as

where the donor density is assumed to be constant.

d 2VRdx2

= !q ND!

(0 " x " w)

Here, the boundary conditions are 0=x

!

V(0) = 0

!

x = wV (w) =Vbi +VR, dV (w)dx

= 0

Therefore, the depletion layer width w can be determined by

w = 2!(Vbi +VR )qND

C = !w=

q!ND2(Vbi +VR )

Depletion layer capacity C is

qND

w x

Charge distributions

w x

Electric field distributions

Depletion layer

EF

qVR EC

EV

w x

Potential distributions

at

at

* www.tc.knct.ac.jp/~hayama/denshi/chapter3.ppt

Ohmic Contact By highly doping an interfacial region :

* S. Kishino, Physics of Semiconductor Devices (Maruzen, Tokyo, 1995).

Vacuum level

Vacuum level

Metal ( ) semiconductor Semiconductor

Junction

• 7

Realistic Schottky Barrier Image force and Shottky barrier :

* S. M. Sze, Physics of Semiconductor Devices (Wiley, New York, 2006).

Exercise 6

Calculate the depletion layer capacity at a reverse bias

VR = 0.5 V in a Au/n-Si Schottky diode. Assume the

following parameters:

Au work function: M = 4.80 eV

n-region: doping density of ND = 1 1021 m-3

Si electron affinity: = 4.05 eV

Si Fermi level: EF = EC 0.15 eV

permittivity: = 0 = 12.0 8.854 10-12 F/m

and q = 1.6 10-19 C.

q(Vbi + VR )

Depletion layer

EF

qVR EC

EV